Simulations of sub-100nm strained Si MOSFETs with high- gate stacks. Lianfeng Yang , Jeremy Watling * , Fikru Adamu-Lema , Asen Asenov and John Barker Device Modelling Group, University of Glasgow Tel: +44-141-330 5343 Fax: +44-141-330 4907 Email: [email protected]
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Lianfeng Yang, Jeremy Watling*, Fikru Adamu-Lema,
Asen Asenov and John Barker
Device Modelling Group,
University of Glasgow
Tel: +44-141-330 5343 Fax: +44-141-330 4907
Email: [email protected]
10th International Workshop on
Computational Electronics (IWCE-10)
24th - 27th October 2004
From ITRS 2003 edition
Our ensemble Monte Carlo simulator includes all relevant scattering mechanisms:
optical intervalley phonon, inelastic acoustic phonon, ionized impurity,
along with interface roughness scattering. The simulator has been thoroughly calibrated for bulk Si transport.
Monte-Carlo calculation of the low-field in- and out-of-plane electron mobilities in strained Si as a function of Ge content within the SiGe buffer; inset shows the in and out-of-plane directions.
Source: IBM (VLSI 2002)
In the strained Si MOSFET:
(Ge content: 15%)
K.Rim, et. al., Symposium on VLSI Technology 2001
Comparison between the n-type Strained Si and control Si MOSFETs:
(Ge content: 15%)
Calibrated ID-VG characteristics of the 67nm n-type bulk Si and strained Si MOSFETs (experimental data from Rim VLSI’01)
† L. Yang, et al, ‘Si/SiGe Heterostructure Parameters for Device Simulations’,to Semiconductor Science and Technology 19, p. 1174-1182 (2004)
Calibrated ID-VG characteristics for 67nm conventional Si and strained MOSFETs, comparison with experimental data of Rim.
Smoother interface for strained Si/SiO2 interface.
See L. Yang et al, Proceedings of the 5th European Workshop on Ultimate Integration of Silicon (ULIS04), p23-26, IMEC 2004
Problems associated with high- dielectrics
“Ideal” high- films: thermally stable, free from electron and interface traps, leakage-free, reliable and reproducible, etc.
Electronic polarization 1/Eg
Highly polarized “soft” metal-oxygen bonds
which screen external fields low energy lattice oscillation (soft - phonon energy)
High dielectric constant
Coupling strength between the inversion layer electrons and the soft optical (SO) phonons (from the LO modes of insulator) Fröhlich interaction
Optical (high frequency)
SiO2 – small difference between and
High- – large difference between and
Strong SO phonon scattering degrades the inversion layer carrier mobility within the MOSFET with high- gate stacks.
ID-VG characteristics of 67nm n-type Si MOSFET, with and without soft-optical phonon scattering from the HfO2 oxide.
Si MOSFET with HfO2
ID-VG characteristics of 67nm n-type strained Si MOSFET with and without soft-optical phonon scattering from the HfO2 oxide.
Average channel velocities for the 67nm n-type bulk and strained Si MOSFETs, with and without soft-optical phonon scattering from the HfO2 gate stack.
ID-VG characteristics of 67nm n-type Si MOSFET, with and without soft-optical phonon scattering, from the Al2O3 oxide.
Source: Intel, IEDM 2003